#------------------------------------------------------------------------------
#$Date: 2016-03-23 02:33:46 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179188 $
#$URL: svn://www.crystallography.net/cod/cif/4/31/32/4313218.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4313218
loop_
_publ_author_name
'Mark G. Morgan'
'Meitian Wang'
'Wing Yan Chan'
'Arthur Mar'
_publ_contact_author_address
; Department of Chemistry
   University of Alberta
   Edmonton, AB
   Canada  T6G 2G2
;
_publ_contact_author_email       arthur.mar@ualberta.ca
_publ_contact_author_fax         '(780) 492-8231'
_publ_contact_author_name        'Dr. Arthur Mar'
_publ_contact_author_phone       '(780) 492-5592'
_publ_section_title
;
 Lanthanum Gallium Bismuthide, LaGaBi2
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              1549
_journal_page_last               1555
_journal_paper_doi               10.1021/ic020413w
_journal_volume                  42
_journal_year                    2003
_chemical_formula_sum            'Bi2 Ga La'
_chemical_formula_weight         626.59
_chemical_name_common            'lanthanum gallium bismuthide'
_chemical_name_systematic        'lanthanum gallium bismuthide'
_space_group_IT_number           191
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6 2'
_symmetry_space_group_name_H-M   'P 6/m m m'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_date             'April 24, 2002'
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            6
_cell_length_a                   13.5483(4)
_cell_length_b                   13.5483(4)
_cell_length_c                   4.39370(10)
_cell_measurement_reflns_used    3708
_cell_measurement_temperature    295(2)
_cell_measurement_theta_max      32.585
_cell_measurement_theta_min      3.007
_cell_volume                     698.44(3)
_computing_cell_refinement       'Bruker SAINT 6.02 (Bruker, 2000)'
_computing_data_collection       'Bruker SMART 5.051 (Bruker, 1997)'
_computing_data_reduction        'Bruker SAINT 6.02 (Bruker, 2000)'
_computing_molecular_graphics    'ATOMS 5.1 (Dowty, 1999)'
_computing_publication_material  'Bruker SHELXTL 5.1 (Sheldrick, 1997)'
_computing_structure_refinement  'Bruker SHELXTL 5.1 (Sheldrick, 1997)'
_computing_structure_solution    'Bruker SHELXTL 5.1 (Sheldrick, 1997)'
_diffrn_ambient_temperature      295(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Bruker Platform/SMART 1000 CCD'
_diffrn_measurement_method       'ω scan (0.2 deg)'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0778
_diffrn_reflns_av_sigmaI/netI    0.0252
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       6
_diffrn_reflns_limit_l_min       -6
_diffrn_reflns_number            10336
_diffrn_reflns_theta_full        32.59
_diffrn_reflns_theta_max         32.59
_diffrn_reflns_theta_min         1.74
_exptl_absorpt_coefficient_mu    89.857
_exptl_absorpt_correction_T_max  0.2362
_exptl_absorpt_correction_T_min  0.0258
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'Bruker SHELXTL 5.1 (Sheldrick, 1997)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    8.938
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       needle
_exptl_crystal_F_000             1524
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.03
_exptl_crystal_size_min          0.03
_refine_diff_density_max         4.974
_refine_diff_density_min         -3.586
_refine_diff_density_rms         1.168
_refine_ls_extinction_coef       0.00238(16)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.165
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     21
_refine_ls_number_reflns         557
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.165
_refine_ls_R_factor_all          0.0440
_refine_ls_R_factor_gt           0.0369
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0412P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0742
_refine_ls_wR_factor_ref         0.0761
_reflns_number_gt                477
_reflns_number_total             557
_reflns_threshold_expression     I>2σ(I)
_cod_data_source_file            ic020413w.cif
_cod_data_source_block           p6mmm
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'not measured' was changed to '?'
- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 3008 2015-01-20 13:52:24Z robertas 
;
_cod_database_code               4313218
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -y, z'
'y, -x+y, z'
'x-y, x, z'
'y, x, -z'
'x-y, -y, -z'
'-x, -x+y, -z'
'-y, -x, -z'
'-x+y, y, -z'
'x, x-y, -z'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'x, y, -z'
'-y, x-y, -z'
'-x+y, -x, -z'
'-y, -x, z'
'-x+y, y, z'
'x, x-y, z'
'y, x, z'
'x-y, -y, z'
'-x, -x+y, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
La La 0.22530(3) 0.45059(6) 0.5000 0.0091(2) Uani 1 4 d S . .
Ga Ga 0.18199(13) 0.0000 0.5000 0.0219(4) Uani 1 4 d S . .
Bi1 Bi 0.32457(5) 0.0000 0.0000 0.01279(16) Uani 1 4 d S . .
Bi2 Bi 0.5000 0.0000 0.5000 0.0143(2) Uani 1 8 d S . .
Bi3 Bi 0.3333 0.6667 0.0000 0.0097(2) Uani 1 12 d S . .
Bi4 Bi 0.0000 0.0000 0.0000 0.0176(3) Uani 1 24 d S . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ga Ga 0.2307 1.6083 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
La La -0.2871 2.4523 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Bi Bi -4.1077 10.2566 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Bi3 La Bi3 81.819(17) 1_556 . ?
Bi3 La Ga 134.733(11) 1_556 2 ?
Bi3 La Ga 134.733(11) . 2 ?
Bi3 La Ga 134.733(11) 1_556 15_556 ?
Bi3 La Ga 134.733(11) . 15_556 ?
Ga La Ga 42.73(5) 2 15_556 ?
Bi3 La Bi2 82.675(10) 1_556 3_665 ?
Bi3 La Bi2 82.675(10) . 3_665 ?
Ga La Bi2 121.08(3) 2 3_665 ?
Ga La Bi2 78.35(3) 15_556 3_665 ?
Bi3 La Bi2 82.675(10) 1_556 2 ?
Bi3 La Bi2 82.675(10) . 2 ?
Ga La Bi2 78.35(3) 2 2 ?
Ga La Bi2 121.08(3) 15_556 2 ?
Bi2 La Bi2 160.57(2) 3_665 2 ?
Bi3 La Bi1 137.958(14) 1_556 2 ?
Bi3 La Bi1 84.646(8) . 2 ?
Ga La Bi1 50.743(18) 2 2 ?
Ga La Bi1 80.37(2) 15_556 2 ?
Bi2 La Bi1 134.597(10) 3_665 2 ?
Bi2 La Bi1 56.141(9) 2 2 ?
Bi3 La Bi1 137.958(14) 1_556 15 ?
Bi3 La Bi1 84.646(8) . 15 ?
Ga La Bi1 80.37(2) 2 15 ?
Ga La Bi1 50.743(18) 15_556 15 ?
Bi2 La Bi1 56.141(9) 3_665 15 ?
Bi2 La Bi1 134.597(10) 2 15 ?
Bi1 La Bi1 79.404(17) 2 15 ?
Bi3 La Bi1 84.646(8) 1_556 15_556 ?
Bi3 La Bi1 137.958(14) . 15_556 ?
Ga La Bi1 80.37(2) 2 15_556 ?
Ga La Bi1 50.743(18) 15_556 15_556 ?
Bi2 La Bi1 56.141(9) 3_665 15_556 ?
Bi2 La Bi1 134.597(10) 2 15_556 ?
Bi1 La Bi1 129.11(3) 2 15_556 ?
Bi1 La Bi1 79.325(9) 15 15_556 ?
Bi3 La Bi1 84.646(8) 1_556 2_556 ?
Bi3 La Bi1 137.958(14) . 2_556 ?
Ga La Bi1 50.743(18) 2 2_556 ?
Ga La Bi1 80.37(2) 15_556 2_556 ?
Bi2 La Bi1 134.597(10) 3_665 2_556 ?
Bi2 La Bi1 56.141(9) 2 2_556 ?
Bi1 La Bi1 79.325(9) 2 2_556 ?
Bi1 La Bi1 129.11(3) 15 2_556 ?
Bi1 La Bi1 79.404(17) 15_556 2_556 ?
Ga Ga Ga 120.0 14_556 15_556 ?
Ga Ga Bi1 109.278(11) 14_556 1_556 ?
Ga Ga Bi1 109.278(11) 15_556 1_556 ?
Ga Ga Bi1 109.278(11) 14_556 . ?
Ga Ga Bi1 109.278(11) 15_556 . ?
Bi1 Ga Bi1 97.35(6) 1_556 . ?
Ga Ga Bi4 68.079(7) 14_556 . ?
Ga Ga Bi4 68.079(7) 15_556 . ?
Bi1 Ga Bi4 173.02(5) 1_556 . ?
Bi1 Ga Bi4 89.624(11) . . ?
Ga Ga Bi4 68.079(7) 14_556 1_556 ?
Ga Ga Bi4 68.079(7) 15_556 1_556 ?
Bi1 Ga Bi4 89.624(11) 1_556 1_556 ?
Bi1 Ga Bi4 173.02(5) . 1_556 ?
Bi4 Ga Bi4 83.40(4) . 1_556 ?
Ga Ga La 171.37(2) 14_556 14_556 ?
Ga Ga La 68.63(2) 15_556 14_556 ?
Bi1 Ga La 65.65(3) 1_556 14_556 ?
Bi1 Ga La 65.65(3) . 14_556 ?
Bi4 Ga La 117.786(7) . 14_556 ?
Bi4 Ga La 117.786(7) 1_556 14_556 ?
Ga Ga La 68.63(2) 14_556 3 ?
Ga Ga La 171.37(2) 15_556 3 ?
Bi1 Ga La 65.65(3) 1_556 3 ?
Bi1 Ga La 65.65(3) . 3 ?
Bi4 Ga La 117.786(7) . 3 ?
Bi4 Ga La 117.786(7) 1_556 3 ?
La Ga La 102.73(5) 14_556 3 ?
Ga Bi1 Ga 97.35(6) 1_554 . ?
Ga Bi1 Bi2 174.07(3) 1_554 . ?
Ga Bi1 Bi2 88.58(3) . . ?
Ga Bi1 Bi2 88.58(3) 1_554 1_554 ?
Ga Bi1 Bi2 174.07(3) . 1_554 ?
Bi2 Bi1 Bi2 85.493(15) . 1_554 ?
Ga Bi1 La 120.937(18) 1_554 14_556 ?
Ga Bi1 La 63.605(17) . 14_556 ?
Bi2 Bi1 La 61.843(8) . 14_556 ?
Bi2 Bi1 La 113.238(17) 1_554 14_556 ?
Ga Bi1 La 63.605(17) 1_554 3_554 ?
Ga Bi1 La 120.937(18) . 3_554 ?
Bi2 Bi1 La 113.238(17) . 3_554 ?
Bi2 Bi1 La 61.843(8) 1_554 3_554 ?
La Bi1 La 173.96(3) 14_556 3_554 ?
Ga Bi1 La 63.605(17) 1_554 14 ?
Ga Bi1 La 120.937(18) . 14 ?
Bi2 Bi1 La 113.238(17) . 14 ?
Bi2 Bi1 La 61.843(8) 1_554 14 ?
La Bi1 La 79.325(9) 14_556 14 ?
La Bi1 La 100.352(7) 3_554 14 ?
Ga Bi1 La 120.937(18) 1_554 3 ?
Ga Bi1 La 63.605(17) . 3 ?
Bi2 Bi1 La 61.843(8) . 3 ?
Bi2 Bi1 La 113.238(17) 1_554 3 ?
La Bi1 La 100.352(7) 14_556 3 ?
La Bi1 La 79.325(9) 3_554 3 ?
La Bi1 La 173.96(3) 14 3 ?
Bi1 Bi2 Bi1 180.0 . 13_656 ?
Bi1 Bi2 Bi1 85.493(15) . 1_556 ?
Bi1 Bi2 Bi1 94.507(15) 13_656 1_556 ?
Bi1 Bi2 Bi1 94.507(15) . 13_655 ?
Bi1 Bi2 Bi1 85.493(15) 13_656 13_655 ?
Bi1 Bi2 Bi1 180.0 1_556 13_655 ?
Bi1 Bi2 La 62.017(9) . 3 ?
Bi1 Bi2 La 117.983(9) 13_656 3 ?
Bi1 Bi2 La 62.017(9) 1_556 3 ?
Bi1 Bi2 La 117.983(9) 13_655 3 ?
Bi1 Bi2 La 117.983(9) . 15_656 ?
Bi1 Bi2 La 62.017(9) 13_656 15_656 ?
Bi1 Bi2 La 117.983(9) 1_556 15_656 ?
Bi1 Bi2 La 62.017(9) 13_655 15_656 ?
La Bi2 La 180.0 3 15_656 ?
Bi1 Bi2 La 117.983(9) . 2_655 ?
Bi1 Bi2 La 62.017(9) 13_656 2_655 ?
Bi1 Bi2 La 117.983(9) 1_556 2_655 ?
Bi1 Bi2 La 62.017(9) 13_655 2_655 ?
La Bi2 La 79.43(2) 3 2_655 ?
La Bi2 La 100.57(2) 15_656 2_655 ?
Bi1 Bi2 La 62.017(9) . 14_556 ?
Bi1 Bi2 La 117.983(9) 13_656 14_556 ?
Bi1 Bi2 La 62.017(9) 1_556 14_556 ?
Bi1 Bi2 La 117.983(9) 13_655 14_556 ?
La Bi2 La 100.57(2) 3 14_556 ?
La Bi2 La 79.43(2) 15_656 14_556 ?
La Bi2 La 180.00(2) 2_655 14_556 ?
La Bi3 La 81.819(17) 3_565 3_564 ?
La Bi3 La 81.763(13) 3_565 2_665 ?
La Bi3 La 135.596(6) 3_564 2_665 ?
La Bi3 La 135.596(6) 3_565 1_554 ?
La Bi3 La 81.763(13) 3_564 1_554 ?
La Bi3 La 135.596(6) 2_665 1_554 ?
La Bi3 La 135.596(6) 3_565 2_664 ?
La Bi3 La 81.763(13) 3_564 2_664 ?
La Bi3 La 81.819(17) 2_665 2_664 ?
La Bi3 La 81.763(13) 1_554 2_664 ?
La Bi3 La 81.763(13) 3_565 . ?
La Bi3 La 135.596(6) 3_564 . ?
La Bi3 La 81.763(13) 2_665 . ?
La Bi3 La 81.819(17) 1_554 . ?
La Bi3 La 135.596(6) 2_664 . ?
Ga Bi4 Ga 180.00(6) 3_554 15_556 ?
Ga Bi4 Ga 43.841(15) 3_554 14 ?
Ga Bi4 Ga 136.159(15) 15_556 14 ?
Ga Bi4 Ga 43.841(15) 3_554 13 ?
Ga Bi4 Ga 136.159(15) 15_556 13 ?
Ga Bi4 Ga 80.57(3) 14 13 ?
Ga Bi4 Ga 136.159(15) 3_554 . ?
Ga Bi4 Ga 43.841(15) 15_556 . ?
Ga Bi4 Ga 99.43(3) 14 . ?
Ga Bi4 Ga 180.00(4) 13 . ?
Ga Bi4 Ga 136.159(15) 3_554 2 ?
Ga Bi4 Ga 43.841(15) 15_556 2 ?
Ga Bi4 Ga 180.00(4) 14 2 ?
Ga Bi4 Ga 99.43(3) 13 2 ?
Ga Bi4 Ga 80.57(3) . 2 ?
Ga Bi4 Ga 83.40(4) 3_554 3 ?
Ga Bi4 Ga 96.60(4) 15_556 3 ?
Ga Bi4 Ga 99.43(3) 14 3 ?
Ga Bi4 Ga 99.43(3) 13 3 ?
Ga Bi4 Ga 80.57(3) . 3 ?
Ga Bi4 Ga 80.57(3) 2 3 ?
Ga Bi4 Ga 99.43(3) 3_554 13_556 ?
Ga Bi4 Ga 80.57(3) 15_556 13_556 ?
Ga Bi4 Ga 136.159(15) 14 13_556 ?
Ga Bi4 Ga 83.40(4) 13 13_556 ?
Ga Bi4 Ga 96.60(4) . 13_556 ?
Ga Bi4 Ga 43.841(15) 2 13_556 ?
Ga Bi4 Ga 43.841(15) 3 13_556 ?
Ga Bi4 Ga 99.43(3) 3_554 14_556 ?
Ga Bi4 Ga 80.57(3) 15_556 14_556 ?
Ga Bi4 Ga 83.40(4) 14 14_556 ?
Ga Bi4 Ga 136.159(15) 13 14_556 ?
Ga Bi4 Ga 43.841(15) . 14_556 ?
Ga Bi4 Ga 96.60(4) 2 14_556 ?
Ga Bi4 Ga 43.841(15) 3 14_556 ?
Ga Bi4 Ga 80.57(3) 13_556 14_556 ?
Ga Bi4 Ga 96.60(4) 3_554 15 ?
Ga Bi4 Ga 83.40(4) 15_556 15 ?
Ga Bi4 Ga 80.57(3) 14 15 ?
Ga Bi4 Ga 80.57(3) 13 15 ?
Ga Bi4 Ga 99.43(3) . 15 ?
Ga Bi4 Ga 99.43(3) 2 15 ?
Ga Bi4 Ga 180.00(12) 3 15 ?
Ga Bi4 Ga 136.159(15) 13_556 15 ?
Ga Bi4 Ga 136.159(15) 14_556 15 ?
Ga Bi4 Ga 80.57(3) 3_554 1_554 ?
Ga Bi4 Ga 99.43(3) 15_556 1_554 ?
Ga Bi4 Ga 43.841(15) 14 1_554 ?
Ga Bi4 Ga 96.60(4) 13 1_554 ?
Ga Bi4 Ga 83.40(4) . 1_554 ?
Ga Bi4 Ga 136.159(15) 2 1_554 ?
Ga Bi4 Ga 136.159(15) 3 1_554 ?
Ga Bi4 Ga 180.00(4) 13_556 1_554 ?
Ga Bi4 Ga 99.43(3) 14_556 1_554 ?
Ga Bi4 Ga 43.841(15) 15 1_554 ?
Ga Bi4 Ga 80.57(3) 3_554 2_554 ?
Ga Bi4 Ga 99.43(3) 15_556 2_554 ?
Ga Bi4 Ga 96.60(4) 14 2_554 ?
Ga Bi4 Ga 43.841(15) 13 2_554 ?
Ga Bi4 Ga 136.159(15) . 2_554 ?
Ga Bi4 Ga 83.40(4) 2 2_554 ?
Ga Bi4 Ga 136.159(15) 3 2_554 ?
Ga Bi4 Ga 99.43(3) 13_556 2_554 ?
Ga Bi4 Ga 180.00(4) 14_556 2_554 ?
Ga Bi4 Ga 43.841(15) 15 2_554 ?
Ga Bi4 Ga 80.57(3) 1_554 2_554 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
La Bi3 3.3547(6) 1_556 ?
La Bi3 3.3547(6) . ?
La Ga 3.3840(13) 2 ?
La Ga 3.3840(13) 15_556 ?
La Bi2 3.43633(16) 3_665 ?
La Bi2 3.43633(16) 2 ?
La Bi1 3.4419(3) 2 ?
La Bi1 3.4419(3) 15 ?
La Bi1 3.4419(3) 15_556 ?
La Bi1 3.4419(3) 2_556 ?
Ga Ga 2.4657(18) 14_556 ?
Ga Ga 2.4657(18) 15_556 ?
Ga Bi1 2.9253(13) 1_556 ?
Ga Bi1 2.9253(13) . ?
Ga Bi4 3.3024(13) . ?
Ga Bi4 3.3024(13) 1_556 ?
Ga La 3.3840(13) 14_556 ?
Ga La 3.3840(13) 3 ?
Bi1 Ga 2.9253(13) 1_554 ?
Bi1 Bi2 3.2366(5) . ?
Bi1 Bi2 3.2366(5) 1_554 ?
Bi1 La 3.4419(3) 14_556 ?
Bi1 La 3.4419(3) 3_554 ?
Bi1 La 3.4419(3) 14 ?
Bi1 La 3.4419(3) 3 ?
Bi2 Bi1 3.2366(5) 13_656 ?
Bi2 Bi1 3.2366(5) 1_556 ?
Bi2 Bi1 3.2366(5) 13_655 ?
Bi2 La 3.43633(16) 3 ?
Bi2 La 3.43633(16) 15_656 ?
Bi2 La 3.43633(16) 2_655 ?
Bi2 La 3.43633(16) 14_556 ?
Bi3 La 3.3547(6) 3_565 ?
Bi3 La 3.3547(6) 3_564 ?
Bi3 La 3.3547(6) 2_665 ?
Bi3 La 3.3547(6) 1_554 ?
Bi3 La 3.3547(6) 2_664 ?
Bi4 Ga 3.3024(13) 3_554 ?
Bi4 Ga 3.3024(13) 15_556 ?
Bi4 Ga 3.3024(13) 14 ?
Bi4 Ga 3.3024(13) 13 ?
Bi4 Ga 3.3024(13) 2 ?
Bi4 Ga 3.3024(13) 3 ?
Bi4 Ga 3.3024(13) 13_556 ?
Bi4 Ga 3.3024(13) 14_556 ?
Bi4 Ga 3.3024(13) 15 ?
Bi4 Ga 3.3024(13) 1_554 ?
Bi4 Ga 3.3024(13) 2_554 ?
